#------------------------------------------------------------------------------
#$Date: 2016-03-25 12:37:44 +0100 (vie 25 de mar de 2016) $
#$Revision: 179854 $
#$URL: svn://www.crystallography.net/cod/cif/7/01/50/7015072.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_7015072
loop_
_publ_author_name
'Zang, Hong-Ying'
'Lan, Ya-Qian'
'Li, Shun-Li'
'Yang, Guang-Sheng'
'Shao, Kui-Zhan'
'Wang, Xin-Long'
'Yan, Li-Kai'
'Su, Zhong-Min'
_publ_section_title
;
 Step-wise synthesis of inorganic-organic hybrid based on
 γ-octamolybdate-based tectons.
;
_journal_issue                   13
_journal_name_full
'Dalton transactions (Cambridge, England : 2003)'
_journal_page_first              3176
_journal_page_last               3182
_journal_paper_doi               10.1039/c0dt00656d
_journal_volume                  40
_journal_year                    2011
_chemical_formula_moiety         'C16 H20 Mo8 N8 O26, 4(H2O)'
_chemical_formula_sum            'C16 H28 Mo8 N8 O30'
_chemical_formula_weight         1579.92
_chemical_name_systematic
;
?
;
_space_group_IT_number           2
_symmetry_cell_setting           triclinic
_symmetry_space_group_name_Hall  '-P 1'
_symmetry_space_group_name_H-M   'P -1'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                102.647(2)
_cell_angle_beta                 113.809(2)
_cell_angle_gamma                108.044(2)
_cell_formula_units_Z            1
_cell_length_a                   10.1710(14)
_cell_length_b                   10.6600(15)
_cell_length_c                   10.9980(15)
_cell_measurement_reflns_used    'total reflection'
_cell_measurement_temperature    293(2)
_cell_measurement_theta_max      26.04
_cell_measurement_theta_min      1.33
_cell_volume                     952.8(2)
_computing_cell_refinement       'Bruker SMART'
_computing_data_collection       'Bruker SMART'
_computing_data_reduction        'Bruker SMART'
_computing_molecular_graphics    'Bruker SHELXTL'
_computing_publication_material  'Bruker SHELXTL'
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_diffrn_ambient_temperature      293(2)
_diffrn_measured_fraction_theta_full 0.982
_diffrn_measured_fraction_theta_max 0.982
_diffrn_measurement_device_type  'Bruker SMART APEX II CCD area-detector'
_diffrn_measurement_method       'φ and ω scans'
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71069
_diffrn_reflns_av_R_equivalents  0.0182
_diffrn_reflns_av_sigmaI/netI    0.0378
_diffrn_reflns_limit_h_max       10
_diffrn_reflns_limit_h_min       -12
_diffrn_reflns_limit_k_max       12
_diffrn_reflns_limit_k_min       -8
_diffrn_reflns_limit_l_max       13
_diffrn_reflns_limit_l_min       -13
_diffrn_reflns_number            4774
_diffrn_reflns_theta_full        25.00
_diffrn_reflns_theta_max         25.00
_diffrn_reflns_theta_min         2.19
_diffrn_standards_interval_time  0
_diffrn_standards_number         0
_exptl_absorpt_coefficient_mu    2.658
_exptl_absorpt_correction_T_max  0.391
_exptl_absorpt_correction_T_min  0.281
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details   'SADABS (Sheldrick, 1996)'
_exptl_crystal_colour            colorless
_exptl_crystal_density_diffrn    2.740
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       block
_exptl_crystal_F_000             748
_exptl_crystal_size_max          0.52
_exptl_crystal_size_mid          0.41
_exptl_crystal_size_min          0.34
_refine_diff_density_max         1.306
_refine_diff_density_min         -0.799
_refine_diff_density_rms         0.158
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.023
_refine_ls_hydrogen_treatment    mixed
_refine_ls_matrix_type           full
_refine_ls_number_parameters     284
_refine_ls_number_reflns         3293
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.023
_refine_ls_R_factor_all          0.0453
_refine_ls_R_factor_gt           0.0363
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[σ²(Fo²)+(0.0574P)²+1.0892P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0907
_refine_ls_wR_factor_ref         0.0964
_reflns_number_gt                2769
_reflns_number_total             3293
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            c0dt00656d.txt
_cod_data_source_block           1
_cod_depositor_comments
;
The following automatic conversions were performed:
'_symmetry_cell_setting' value 'Triclinic' changed to 'triclinic'
according to '/home/saulius/struct/CIF-dictionaries/cif_core.dic'
dictionary named 'cif_core.dic' version 2.4.1 from 2010-06-29.

Automatic conversion script
Id: cif_fix_enum 1555 2011-01-17 13:19:09Z saulius 
;
_cod_original_sg_symbol_H-M      p-1
_cod_database_code               7015072
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-x, -y, -z'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
_atom_site_disorder_assembly
_atom_site_disorder_group
Mo1 Mo 0.96180(6) 0.33873(5) 0.02011(6) 0.01999(15) Uani 1 1 d . . .
Mo2 Mo 0.84158(6) 0.36762(5) -0.31285(6) 0.02344(16) Uani 1 1 d . . .
Mo3 Mo 0.59613(6) 0.33542(6) -0.18903(6) 0.02310(16) Uani 1 1 d . . .
Mo4 Mo 0.70989(6) 0.35810(6) 0.13988(6) 0.02349(16) Uani 1 1 d . . .
C1 C 1.3391(8) 0.2776(7) 0.3852(7) 0.0339(16) Uani 1 1 d . . .
H14 H 1.3337 0.3647 0.4016 0.041 Uiso 1 1 calc R . .
C2 C 1.4297(9) 0.1137(9) 0.2991(8) 0.0461(19) Uani 1 1 d . . .
H20 H 1.4847 0.0899 0.2551 0.055 Uiso 1 1 calc R . .
C3 C 1.3555(7) 0.0234(6) 0.3391(7) 0.0255(14) Uani 1 1 d . . .
H10 H 1.3627 -0.0630 0.3254 0.031 Uiso 1 1 calc R . .
C4 C 1.2705(8) 0.0471(7) 0.3980(8) 0.0368(17) Uani 1 1 d . . .
H12 H 1.2183 -0.0224 0.4226 0.044 Uiso 1 1 calc R . .
C5 C 1.2593(8) 0.1747(7) 0.4231(7) 0.0303(15) Uani 1 1 d . . .
C6 C 1.1620(8) 0.2002(8) 0.4897(8) 0.0348(16) Uani 1 1 d . . .
H10A H 1.1408 0.1306 0.5317 0.042 Uiso 1 1 calc R . .
H10B H 1.2232 0.2952 0.5669 0.042 Uiso 1 1 calc R . .
C7 C 0.9728(8) 0.2936(7) 0.3647(7) 0.0305(15) Uani 1 1 d . . .
H17 H 1.0391 0.3906 0.4232 0.037 Uiso 1 1 calc R . .
C8 C 0.7779(9) 0.0963(7) 0.2036(9) 0.045(2) Uani 1 1 d . . .
H19 H 0.6773 0.0293 0.1253 0.054 Uiso 1 1 calc R . .
N1 N 1.4261(9) 0.2482(8) 0.3230(9) 0.064(2) Uani 1 1 d . . .
N2 N 1.0095(7) 0.1884(6) 0.3832(6) 0.0303(13) Uani 1 1 d . . .
N3 N 0.8870(7) 0.0618(6) 0.2804(7) 0.0488(18) Uani 1 1 d . . .
H3 H 0.8816 -0.0226 0.2679 0.059 Uiso 1 1 calc R . .
N4 N 0.8275(6) 0.2409(6) 0.2504(6) 0.0275(12) Uani 1 1 d . . .
O1 O 0.8554(5) 0.4736(4) -0.1053(4) 0.0228(9) Uani 1 1 d . . .
O2 O 0.8682(6) 0.2514(5) -0.4234(5) 0.0419(13) Uani 1 1 d . . .
O1W O 0.7495(8) 0.7392(7) 0.0961(9) 0.081(2) Uani 1 1 d . . .
O3 O 0.7523(6) 0.4480(5) -0.4151(5) 0.0375(12) Uani 1 1 d . . .
O4 O 0.9549(5) 0.2730(4) -0.1438(4) 0.0249(9) Uani 1 1 d . . .
O5 O 1.0423(5) 0.2495(5) 0.1141(5) 0.0310(10) Uani 1 1 d . . .
O6 O 0.6504(5) 0.2394(4) -0.3204(4) 0.0250(9) Uani 1 1 d . . .
O7 O 0.5410(6) 0.4477(5) -0.2623(5) 0.0346(11) Uani 1 1 d . . .
O8 O 0.4205(5) 0.1933(5) -0.2436(5) 0.0341(11) Uani 1 1 d . . .
O9 O 0.6418(5) 0.4418(4) 0.0060(5) 0.0280(10) Uani 1 1 d . . .
O10 O 0.7441(5) 0.2529(4) -0.0374(4) 0.0224(9) Uani 1 1 d . . .
O11 O 0.5338(5) 0.2109(5) 0.0786(5) 0.0332(11) Uani 1 1 d . . .
O12 O 0.7440(6) 0.4749(5) 0.2939(5) 0.0371(12) Uani 1 1 d . . .
O13 O 0.9490(5) 0.4707(4) 0.1892(4) 0.0236(9) Uani 1 1 d . . .
O2W O 1.119(3) 0.055(2) -0.001(2) 0.293(10) Uani 1 1 d . . .
H1N H 1.483(9) 0.338(8) 0.277(8) 0.06(2) Uiso 1 1 d . . .
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
C C 0.0033 0.0016 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
N N 0.0061 0.0033 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Mo Mo -1.6832 0.6857 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
O5 Mo1 O4 103.4(2) . . ?
O5 Mo1 O10 104.79(19) . . ?
O4 Mo1 O10 101.46(19) . . ?
O5 Mo1 O1 102.48(19) . 2_765 ?
O4 Mo1 O1 97.77(18) . 2_765 ?
O10 Mo1 O1 141.69(18) . 2_765 ?
O5 Mo1 O13 96.44(19) . . ?
O4 Mo1 O13 159.84(17) . . ?
O10 Mo1 O13 76.34(17) . . ?
O1 Mo1 O13 74.31(16) 2_765 . ?
O5 Mo1 O1 177.81(18) . . ?
O4 Mo1 O1 77.92(17) . . ?
O10 Mo1 O1 76.51(15) . . ?
O1 Mo1 O1 75.57(17) 2_765 . ?
O13 Mo1 O1 82.11(15) . . ?
O2 Mo2 O3 105.2(2) . . ?
O2 Mo2 O13 104.4(2) . 2_765 ?
O3 Mo2 O13 97.55(19) . 2_765 ?
O2 Mo2 O6 102.1(2) . . ?
O3 Mo2 O6 97.1(2) . . ?
O13 Mo2 O6 145.07(18) 2_765 . ?
O2 Mo2 O1 154.3(2) . . ?
O3 Mo2 O1 100.5(2) . . ?
O13 Mo2 O1 72.60(16) 2_765 . ?
O6 Mo2 O1 73.65(16) . . ?
O2 Mo2 O4 84.0(2) . . ?
O3 Mo2 O4 170.7(2) . . ?
O13 Mo2 O4 81.67(16) 2_765 . ?
O6 Mo2 O4 78.80(16) . . ?
O1 Mo2 O4 70.37(14) . . ?
O7 Mo3 O8 105.2(2) . . ?
O7 Mo3 O6 102.3(2) . . ?
O8 Mo3 O6 96.9(2) . . ?
O7 Mo3 O9 95.7(2) . . ?
O8 Mo3 O9 98.0(2) . . ?
O6 Mo3 O9 152.71(18) . . ?
O7 Mo3 O1 91.41(19) . . ?
O8 Mo3 O1 162.6(2) . . ?
O6 Mo3 O1 73.92(16) . . ?
O9 Mo3 O1 85.39(17) . . ?
O7 Mo3 O10 161.19(19) . . ?
O8 Mo3 O10 91.95(19) . . ?
O6 Mo3 O10 82.91(16) . . ?
O9 Mo3 O10 73.87(16) . . ?
O1 Mo3 O10 72.47(14) . . ?
O12 Mo4 O11 105.4(2) . . ?
O12 Mo4 O9 102.6(2) . . ?
O11 Mo4 O9 101.3(2) . . ?
O12 Mo4 O13 92.3(2) . . ?
O11 Mo4 O13 156.7(2) . . ?
O9 Mo4 O13 89.28(17) . . ?
O12 Mo4 N4 94.0(2) . . ?
O11 Mo4 N4 85.1(2) . . ?
O9 Mo4 N4 159.68(19) . . ?
O13 Mo4 N4 78.44(17) . . ?
O12 Mo4 O10 161.97(19) . . ?
O11 Mo4 O10 92.30(19) . . ?
O9 Mo4 O10 76.71(16) . . ?
O13 Mo4 O10 69.76(15) . . ?
N4 Mo4 O10 83.83(17) . . ?
N1 C1 C5 119.2(7) . . ?
N1 C1 H14 120.4 . . ?
C5 C1 H14 120.4 . . ?
C3 C2 N1 119.6(7) . . ?
C3 C2 H20 120.2 . . ?
N1 C2 H20 120.2 . . ?
C2 C3 C4 123.8(6) . . ?
C2 C3 H10 118.1 . . ?
C4 C3 H10 118.1 . . ?
C3 C4 C5 120.0(6) . . ?
C3 C4 H12 120.0 . . ?
C5 C4 H12 120.0 . . ?
C4 C5 C1 118.9(7) . . ?
C4 C5 C6 119.5(6) . . ?
C1 C5 C6 121.6(6) . . ?
N2 C6 C5 111.8(6) . . ?
N2 C6 H10A 109.3 . . ?
C5 C6 H10A 109.3 . . ?
N2 C6 H10B 109.3 . . ?
C5 C6 H10B 109.3 . . ?
H10A C6 H10B 107.9 . . ?
N2 C7 N4 110.1(6) . . ?
N2 C7 H17 125.0 . . ?
N4 C7 H17 125.0 . . ?
N3 C8 N4 112.8(6) . . ?
N3 C8 H19 123.6 . . ?
N4 C8 H19 123.6 . . ?
C1 N1 C2 118.3(7) . . ?
C1 N1 H1N 117(4) . . ?
C2 N1 H1N 124(4) . . ?
C7 N2 N3 109.7(6) . . ?
C7 N2 C6 127.7(6) . . ?
N3 N2 C6 122.5(5) . . ?
C8 N3 N2 104.1(6) . . ?
C8 N3 H3 127.9 . . ?
N2 N3 H3 127.9 . . ?
C7 N4 C8 103.2(6) . . ?
C7 N4 Mo4 128.4(4) . . ?
C8 N4 Mo4 127.6(5) . . ?
Mo1 O1 Mo3 151.5(2) 2_765 . ?
Mo1 O1 Mo2 102.19(17) 2_765 . ?
Mo3 O1 Mo2 93.38(15) . . ?
Mo1 O1 Mo1 104.43(17) 2_765 . ?
Mo3 O1 Mo1 97.07(14) . . ?
Mo2 O1 Mo1 97.05(15) . . ?
Mo1 O4 Mo2 114.5(2) . . ?
Mo3 O6 Mo2 113.3(2) . . ?
Mo4 O9 Mo3 114.2(2) . . ?
Mo1 O10 Mo4 109.26(18) . . ?
Mo1 O10 Mo3 112.97(18) . . ?
Mo4 O10 Mo3 91.57(15) . . ?
Mo2 O13 Mo4 149.8(2) 2_765 . ?
Mo2 O13 Mo1 106.38(19) 2_765 . ?
Mo4 O13 Mo1 103.77(17) . . ?
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
Mo1 O5 1.696(4) . ?
Mo1 O4 1.749(4) . ?
Mo1 O10 1.871(4) . ?
Mo1 O1 1.951(4) 2_765 ?
Mo1 O13 2.149(4) . ?
Mo1 O1 2.402(4) . ?
Mo2 O2 1.703(5) . ?
Mo2 O3 1.704(5) . ?
Mo2 O13 1.928(4) 2_765 ?
Mo2 O6 1.957(4) . ?
Mo2 O1 2.241(4) . ?
Mo2 O4 2.370(4) . ?
Mo3 O7 1.694(4) . ?
Mo3 O8 1.705(4) . ?
Mo3 O6 1.946(4) . ?
Mo3 O9 1.977(4) . ?
Mo3 O1 2.238(4) . ?
Mo3 O10 2.292(4) . ?
Mo4 O12 1.695(4) . ?
Mo4 O11 1.716(4) . ?
Mo4 O9 1.892(4) . ?
Mo4 O13 2.119(4) . ?
Mo4 N4 2.210(5) . ?
Mo4 O10 2.239(4) . ?
C1 N1 1.385(10) . ?
C1 C5 1.399(9) . ?
C1 H14 0.9300 . ?
C2 C3 1.301(10) . ?
C2 N1 1.414(11) . ?
C2 H20 0.9300 . ?
C3 C4 1.322(10) . ?
C3 H10 0.9300 . ?
C4 C5 1.377(9) . ?
C4 H12 0.9300 . ?
C5 C6 1.502(10) . ?
C6 N2 1.463(8) . ?
C6 H10A 0.9700 . ?
C6 H10B 0.9700 . ?
C7 N2 1.318(8) . ?
C7 N4 1.325(8) . ?
C7 H17 0.9300 . ?
C8 N3 1.309(9) . ?
C8 N4 1.362(8) . ?
C8 H19 0.9300 . ?
N1 H1N 1.27(8) . ?
N2 N3 1.343(8) . ?
N3 H3 0.8600 . ?
O1 Mo1 1.951(4) 2_765 ?
O13 Mo2 1.928(4) 2_765 ?
loop_
_geom_torsion_atom_site_label_1
_geom_torsion_atom_site_label_2
_geom_torsion_atom_site_label_3
_geom_torsion_atom_site_label_4
_geom_torsion
_geom_torsion_site_symmetry_1
_geom_torsion_site_symmetry_2
_geom_torsion_site_symmetry_3
_geom_torsion_site_symmetry_4
_geom_torsion_publ_flag
N1 C2 C3 C4 2.2(11) . . . . ?
C2 C3 C4 C5 -1.3(11) . . . . ?
C3 C4 C5 C1 0.0(10) . . . . ?
C3 C4 C5 C6 179.8(6) . . . . ?
N1 C1 C5 C4 0.4(10) . . . . ?
N1 C1 C5 C6 -179.5(6) . . . . ?
C4 C5 C6 N2 -105.6(7) . . . . ?
C1 C5 C6 N2 74.2(8) . . . . ?
C5 C1 N1 C2 0.5(11) . . . . ?
C3 C2 N1 C1 -1.8(11) . . . . ?
N4 C7 N2 N3 -0.3(8) . . . . ?
N4 C7 N2 C6 175.2(6) . . . . ?
C5 C6 N2 C7 -102.4(8) . . . . ?
C5 C6 N2 N3 72.6(8) . . . . ?
N4 C8 N3 N2 1.9(9) . . . . ?
C7 N2 N3 C8 -1.0(8) . . . . ?
C6 N2 N3 C8 -176.8(7) . . . . ?
N2 C7 N4 C8 1.4(8) . . . . ?
N2 C7 N4 Mo4 -169.4(4) . . . . ?
N3 C8 N4 C7 -2.1(9) . . . . ?
N3 C8 N4 Mo4 168.8(5) . . . . ?
O12 Mo4 N4 C7 -52.4(6) . . . . ?
O11 Mo4 N4 C7 -157.5(6) . . . . ?
O9 Mo4 N4 C7 93.0(8) . . . . ?
O13 Mo4 N4 C7 39.1(6) . . . . ?
O10 Mo4 N4 C7 109.6(6) . . . . ?
O12 Mo4 N4 C8 139.0(6) . . . . ?
O11 Mo4 N4 C8 33.9(6) . . . . ?
O9 Mo4 N4 C8 -75.6(8) . . . . ?
O13 Mo4 N4 C8 -129.5(6) . . . . ?
O10 Mo4 N4 C8 -58.9(6) . . . . ?
O7 Mo3 O1 Mo1 37.5(5) . . . 2_765 ?
O8 Mo3 O1 Mo1 -160.2(6) . . . 2_765 ?
O6 Mo3 O1 Mo1 139.9(5) . . . 2_765 ?
O9 Mo3 O1 Mo1 -58.1(4) . . . 2_765 ?
O10 Mo3 O1 Mo1 -132.6(5) . . . 2_765 ?
O7 Mo3 O1 Mo2 -86.0(2) . . . . ?
O8 Mo3 O1 Mo2 76.3(7) . . . . ?
O6 Mo3 O1 Mo2 16.38(15) . . . . ?
O9 Mo3 O1 Mo2 178.39(16) . . . . ?
O10 Mo3 O1 Mo2 103.87(17) . . . . ?
O7 Mo3 O1 Mo1 176.5(2) . . . . ?
O8 Mo3 O1 Mo1 -21.3(7) . . . . ?
O6 Mo3 O1 Mo1 -81.16(17) . . . . ?
O9 Mo3 O1 Mo1 80.85(16) . . . . ?
O10 Mo3 O1 Mo1 6.33(13) . . . . ?
O2 Mo2 O1 Mo1 103.9(5) . . . 2_765 ?
O3 Mo2 O1 Mo1 -77.8(2) . . . 2_765 ?
O13 Mo2 O1 Mo1 16.88(17) 2_765 . . 2_765 ?
O6 Mo2 O1 Mo1 -172.3(2) . . . 2_765 ?
O4 Mo2 O1 Mo1 104.06(19) . . . 2_765 ?
O2 Mo2 O1 Mo3 -100.1(5) . . . . ?
O3 Mo2 O1 Mo3 78.14(19) . . . . ?
O13 Mo2 O1 Mo3 172.9(2) 2_765 . . . ?
O6 Mo2 O1 Mo3 -16.31(15) . . . . ?
O4 Mo2 O1 Mo3 -99.98(16) . . . . ?
O2 Mo2 O1 Mo1 -2.6(5) . . . . ?
O3 Mo2 O1 Mo1 175.70(17) . . . . ?
O13 Mo2 O1 Mo1 -89.59(17) 2_765 . . . ?
O6 Mo2 O1 Mo1 81.25(17) . . . . ?
O4 Mo2 O1 Mo1 -2.42(12) . . . . ?
O5 Mo1 O1 Mo1 27(5) . . . 2_765 ?
O4 Mo1 O1 Mo1 -101.4(2) . . . 2_765 ?
O10 Mo1 O1 Mo1 153.5(2) . . . 2_765 ?
O1 Mo1 O1 Mo1 0.0 2_765 . . 2_765 ?
O13 Mo1 O1 Mo1 75.74(19) . . . 2_765 ?
O5 Mo1 O1 Mo3 -134(5) . . . . ?
O4 Mo1 O1 Mo3 97.48(18) . . . . ?
O10 Mo1 O1 Mo3 -7.62(15) . . . . ?
O1 Mo1 O1 Mo3 -161.1(3) 2_765 . . . ?
O13 Mo1 O1 Mo3 -85.37(16) . . . . ?
O5 Mo1 O1 Mo2 131(5) . . . . ?
O4 Mo1 O1 Mo2 3.16(16) . . . . ?
O10 Mo1 O1 Mo2 -101.93(18) . . . . ?
O1 Mo1 O1 Mo2 104.6(2) 2_765 . . . ?
O13 Mo1 O1 Mo2 -179.69(16) . . . . ?
O5 Mo1 O4 Mo2 178.5(2) . . . . ?
O10 Mo1 O4 Mo2 70.1(2) . . . . ?
O1 Mo1 O4 Mo2 -76.6(2) 2_765 . . . ?
O13 Mo1 O4 Mo2 -11.5(6) . . . . ?
O1 Mo1 O4 Mo2 -3.26(17) . . . . ?
O2 Mo2 O4 Mo1 -176.4(3) . . . . ?
O3 Mo2 O4 Mo1 -7.9(12) . . . . ?
O13 Mo2 O4 Mo1 78.0(2) 2_765 . . . ?
O6 Mo2 O4 Mo1 -72.8(2) . . . . ?
O1 Mo2 O4 Mo1 3.63(19) . . . . ?
O7 Mo3 O6 Mo2 67.4(3) . . . . ?
O8 Mo3 O6 Mo2 174.6(2) . . . . ?
O9 Mo3 O6 Mo2 -62.7(4) . . . . ?
O1 Mo3 O6 Mo2 -20.55(19) . . . . ?
O10 Mo3 O6 Mo2 -94.3(2) . . . . ?
O2 Mo2 O6 Mo3 174.4(2) . . . . ?
O3 Mo2 O6 Mo3 -78.3(3) . . . . ?
O13 Mo2 O6 Mo3 35.9(4) 2_765 . . . ?
O1 Mo2 O6 Mo3 20.55(19) . . . . ?
O4 Mo2 O6 Mo3 93.2(2) . . . . ?
O12 Mo4 O9 Mo3 178.3(2) . . . . ?
O11 Mo4 O9 Mo3 -72.9(3) . . . . ?
O13 Mo4 O9 Mo3 86.1(2) . . . . ?
N4 Mo4 O9 Mo3 33.8(7) . . . . ?
O10 Mo4 O9 Mo3 16.78(19) . . . . ?
O7 Mo3 O9 Mo4 179.4(2) . . . . ?
O8 Mo3 O9 Mo4 73.1(3) . . . . ?
O6 Mo3 O9 Mo4 -49.4(5) . . . . ?
O1 Mo3 O9 Mo4 -89.7(2) . . . . ?
O10 Mo3 O9 Mo4 -16.60(19) . . . . ?
O5 Mo1 O10 Mo4 85.9(2) . . . . ?
O4 Mo1 O10 Mo4 -166.77(18) . . . . ?
O1 Mo1 O10 Mo4 -48.1(3) 2_765 . . . ?
O13 Mo1 O10 Mo4 -7.31(16) . . . . ?
O1 Mo1 O10 Mo4 -92.33(18) . . . . ?
O5 Mo1 O10 Mo3 -173.8(2) . . . . ?
O4 Mo1 O10 Mo3 -66.4(2) . . . . ?
O1 Mo1 O10 Mo3 52.2(4) 2_765 . . . ?
O13 Mo1 O10 Mo3 93.0(2) . . . . ?
O1 Mo1 O10 Mo3 8.02(16) . . . . ?
O12 Mo4 O10 Mo1 11.9(7) . . . . ?
O11 Mo4 O10 Mo1 -157.0(2) . . . . ?
O9 Mo4 O10 Mo1 101.9(2) . . . . ?
O13 Mo4 O10 Mo1 7.68(17) . . . . ?
N4 Mo4 O10 Mo1 -72.2(2) . . . . ?
O12 Mo4 O10 Mo3 -103.2(6) . . . . ?
O11 Mo4 O10 Mo3 87.93(18) . . . . ?
O9 Mo4 O10 Mo3 -13.14(15) . . . . ?
O13 Mo4 O10 Mo3 -107.34(17) . . . . ?
N4 Mo4 O10 Mo3 172.73(17) . . . . ?
O7 Mo3 O10 Mo1 -40.9(7) . . . . ?
O8 Mo3 O10 Mo1 163.2(2) . . . . ?
O6 Mo3 O10 Mo1 66.5(2) . . . . ?
O9 Mo3 O10 Mo1 -99.0(2) . . . . ?
O1 Mo3 O10 Mo1 -8.78(18) . . . . ?
O7 Mo3 O10 Mo4 70.8(6) . . . . ?
O8 Mo3 O10 Mo4 -85.05(19) . . . . ?
O6 Mo3 O10 Mo4 178.25(16) . . . . ?
O9 Mo3 O10 Mo4 12.73(15) . . . . ?
O1 Mo3 O10 Mo4 102.93(16) . . . . ?
O12 Mo4 O13 Mo2 -4.4(5) . . . 2_765 ?
O11 Mo4 O13 Mo2 -144.0(5) . . . 2_765 ?
O9 Mo4 O13 Mo2 98.2(5) . . . 2_765 ?
N4 Mo4 O13 Mo2 -98.1(5) . . . 2_765 ?
O10 Mo4 O13 Mo2 174.3(5) . . . 2_765 ?
O12 Mo4 O13 Mo1 174.8(2) . . . . ?
O11 Mo4 O13 Mo1 35.2(5) . . . . ?
O9 Mo4 O13 Mo1 -82.58(19) . . . . ?
N4 Mo4 O13 Mo1 81.1(2) . . . . ?
O10 Mo4 O13 Mo1 -6.50(14) . . . . ?
O5 Mo1 O13 Mo2 83.4(2) . . . 2_765 ?
O4 Mo1 O13 Mo2 -86.8(5) . . . 2_765 ?
O10 Mo1 O13 Mo2 -172.9(2) . . . 2_765 ?
O1 Mo1 O13 Mo2 -17.81(17) 2_765 . . 2_765 ?
O1 Mo1 O13 Mo2 -94.96(19) . . . 2_765 ?
O5 Mo1 O13 Mo4 -96.2(2) . . . . ?
O4 Mo1 O13 Mo4 93.6(5) . . . . ?
O10 Mo1 O13 Mo4 7.51(16) . . . . ?
O1 Mo1 O13 Mo4 162.6(2) 2_765 . . . ?
O1 Mo1 O13 Mo4 85.47(17) . . . . ?
